- freely available
Crystals 2013, 3(3), 483-503; doi:10.3390/cryst3030483
Published: 3 September 2013
Abstract: We review recent progress in the development of high birefringence (Δn ≥ 0.12) negative dielectric anisotropy (Δε < 0) liquid crystals (LCs) for direct-view and projection displays. For mobile displays, our UCF-N2 (low viscosity, negative Δε, high Δn) based homogeneous alignment fringe-field switching (called n-FFS) mode exhibits superior performance to p-FFS in transmittance, single gamma curve, cell gap insensitivity, and negligible flexoelectric effect. For projection displays using a vertical alignment liquid-crystal-on-silicon (VA LCOS), our high birefringence UCF-N3 mixture enables a submillisecond gray-to-gray response time, which is essential for color sequential displays without noticeable color breakup. Our low viscosity UCF-N2 also enables multi-domain VA displays to use a thinner cell gap for achieving faster response time.
Negative dielectric anisotropy (Δε = ε// − < 0) liquid crystals (LCs) [1,2], in which the parallel permittivity (ε//) is smaller than the perpendicular one ( ), have been widely used for direct-view and projection displays. The common feature of a negative Δε LC is that lateral polar substituents induce a dipole moment perpendicular to the principal molecular axis [3,4,5]. As described in , there are several approaches to induce polarity perpendicular to the molecular axis, such as (i) using certain polar linking groups (e.g., ester); (ii) adding a polar unit at an axial position of a cyclohexane ring; (iii) positioning polar unit(s) in lateral positions of an aromatic ring; and (iv) using heterocyclic rings with the heteroatom off-axis. However, the off-axis polar group would decrease the aspect ratio of the cylindrical molecular shape and hence tend to disturb the liquid crystal phase stability. Furthermore, the magnitude of the Δε value will generally be much smaller than that of a positive Δε LC. To use multiple polar groups to enhance Δε often causes solubility problems or increases the rotational viscosity. Different off-axis polar groups, such as cyano and fluoro, have been employed to enlarge perpendicular dipole moment. To avoid image flickering , high resistivity is another crucial requirement for obtaining a high voltage-holding-ratio for active matrix liquid crystal displays (LCDs). A sufficiently large Δε helps to lower the driving voltage, which in turn lowers the power consumption of a mobile display. Fluoro group provides an excellent resistivity , modest dipole moment, and low viscosity. Laterally fluorinated liquid crystals , i.e., (2,3) difluorinated biphenyl, terphenyl  and tolane  usually exhibit a high resistivity and a modest Δε.
Most nematic LC devices require surface alignment layers in order to realize their useful electro-optic effect. However, some exceptions exist; for example, without any alignment layer polymer-stabilized blue phase with a negative Δε LC host has been demonstrated recently to possess a negative Kerr constant and submillisecond response time . A negative Δε LC can be used in homogeneous alignment or vertical alignment (VA), depending on the electric field direction. In an in-plane switching (IPS) cell [13,14] or fringe-field switching (FFS) cell [15,16,17], the electric field is mainly in the lateral direction, while in a VA cell [18,19] or multi-domain VA (MVA) cell [20,21], the field is basically in the longitudinal direction. For mobile displays, IPS or FFS is a favored choice because they are more robust to external pressure, which is crucial for touch panels. In comparison with IPS, FFS mode has narrower electrode width and gap to eliminate dead zones so that its optical throughput is higher. Moreover, the capacitor formed by the passivation layer between the pixel and common electrode acts as a storage capacitance. As a result, FFS mode enables a larger aperture ratio, which translates into higher optical efficiency. Recently, it is found that the FFS mode with a negative Δε LC (n-FFS) exhibits several advantages over its p-FFS (FFS mode using a positive Δε LC) counterpart in higher transmittance, single gamma curve, cell gap insensitivity, and weaker flexoelectric effect . A single-domain VA cell has been employed in liquid-crystal-on-silicon (LCOS) for data projectors because of its unprecedented contrast ratio , while MVA is a common choice for wide-view LCD TVs. In this paper, we will review recent progress on the negative Δε and high Δn LC development for mobile displays using FFS mode, projection displays using VA LCOS, and wide-view LCD TVs using MVA. Among these applications, fast response time is a common requirement.
2. Response Time of Negative Δε LCs
Fast response time plays a key role for reducing the image blur and improving transmittance in conventional LCDs, and for realizing color sequential displays without color breakup. The dynamic response of LC directors is governed by Ericksen-Leslie equation. Under single elastic constant and small angle approximations, Ericksen-Leslie equation can be simplified as :
By solving Equation (2), we obtain the free relaxation time of the LC directors:
3. Negative Δε LCs for FFS Mode
FFS [15,32,33] mode has been widely used for mobile displays, such as smartphones and tablet computers. Low power consumption for long battery life, wide viewing angle for multiple observers, high resolution for Retina display, and pressure-resistance for touch screen are the key requirements. In FFS mode, the electric field-induced molecular reorientation takes place mainly in the horizontal direction. Presently, most FFS LCDs use positive Δε LCs. The primary reason is that it is relatively easy to obtain a large Δε (~10) LC while keeping a low viscosity. Large Δε helps to reduce operation voltage while low viscosity helps to shorten response time. However, p-FFS has some problems: (1) its peak transmittance is ~88%; (2) the voltage-dependent transmittance (VT) curves do not overlap well for RGB colors, thus three gamma curves are required, which increases the complexity of driving electronics; (3) the VT curves are sensitive to the cell gap; and (4) a small but noticeable image flickering due to splay- and bend-induced flexoelectric effect [34,35].
To overcome these problems, recently we reported a n-FFS mode using a high performance negative Δε LC . The n-FFS mode has been investigated previously [13,15,17], but mainly by simulations. In this section, we compare the results of four different negative Δε LC mixtures with relatively high Δn and low viscosity. The phase retardation effect on peak transmittance and on-state voltage is also investigated.
3.1. Low Viscosity Negative Δε LCs
For high yield manufacturing, it is desirable to keep the cell gap above 3 μm. Thus, the required Δn is around 0.12. Previously we reported a high performance n-FFS with UCF-N1 , consisting of 60 wt % MLC-6882, 18% lateral difluoro akoxy-biphenyl, 17% lateral difluoro akoxy-cyclohexane-biphenyl  and 5% bicyclohexane compounds. The chemical structures are shown in Figure 1. We compare our results with MLC-6882 and a virtual positive Δε LC (UCF-P1) whose Δε = 10 and other properties are the same as UCF-N1.
In addition to MLC 6882, UCF-N1 and UCF-P1, Table 1 includes three new negative Δε LCs to be considered for FFS mode: HAV (HAV-634117, HCCH, Nanjing, China), ZOC (ZOC-7003, JNC, Ichihara, Japan), and UCF-N2. From Table 1, JNC ZOC has the lowest visco-elastic coefficient γ1/K33, but its Δn ~ 0.1 which is slightly too small. For an LCOS, the panel size is small, thus a submicron cell gap can be controlled without too much difficulty. However, a high Δn LC is needed to maintain dΔn ~ 165 nm. To obtain high Δn, we first formulated a binary LC mixture (M1) with two lateral difluoro-terphenyl homologs: R1 = 2, R2 = 4 (35 wt %) and R1 = 3, R2 = 5 (65 wt %) . The general chemical structure is also shown in Figure 1. Its physical properties are: Δn = 0.235 (at λ = 633 nm and T ~ 22 °C), Δε = −1.8 and clearing temperature Tc ~ 112.3 °C. Next, we doped 10% M1 and 5% biphenyls to ZOC-7003. The final mixture is denoted as UCF-N2. Table 1 lists the physical properties of the six LC mixtures studied. The dielectric anisotropy was determined by measuring the capacitance of a homogeneous cell and a homeotropic LC cell [37,38].
|Table 1. Physical properties of the LCs studied (λ = 633 nm, T ~ 22 °C and f = 1 kHz).|
|LC Mixture||Tc (°C)||Δn (633 nm)||Δn (550 nm)||γ1/K33 (ms/μm2)||γ1 (mPas)||Δε|
We evaluated birefringence by measuring the phase retardation of a VA cell sandwiched between two crossed polarizers . The VA cell has strong anchoring energy and cell gap d ~ 9 µm. A 1 kHz square-wave AC voltage signal was applied to the LC cell. A He-Ne laser (λ = 633 nm) and a tunable Argon ion laser (λ = 457 nm, 488 nm and 514 nm) were used as probing beams. The Δn of UCF-N1, HAV, ZOC and UCF-N2 was measured from 22 °C (RT) to a temperature close to Tc. Results are plotted in Figure 2. Dots represent the measured data and solid lines are the fitting curves using Haller’s semi-empirical equation :
For a full color display, we need to know the birefringence at red, green and blue wavelengths. Figure 3 depicts the measured birefringence dispersion of UCF-N1, HAV, ZOC and UCF-N2. Dots represent measured data and solid lines are fitting curves using the single-band birefringence dispersion model :
From the relaxation time measurement of the VA cell, we can obtain γ1/K33 . We measured γ1/K33 at different temperatures and fitted the experimental results with Equation (6), as shown in Figure 4a:
3.2. Device Configuration
Next, we compare the electro-optic properties of n-FFS and p-FFS modes. We calculated the LC director distribution by a commercial LCD simulator DIMOS.2D and optical transmittance by extended Jones matrix . As will be shown later, the preferred dΔn value for achieving high transmittance at λ = 550 nm and fast response time is ~360 nm for n-FFS and ~380 nm for p-FFS. This difference originates from more efficient LC director reorientation in n-FFS. To make a fair comparison between n-FFS and p-FFS, we use the same electrode width w = 2 μm and gap l = 3 μm, same pretilt angle (2°) but the rubbing angle is 10° and 80° respectively w.r.t. the horizontal axis, as shown in Figure 4a,b. The passivation layer between the pixel and common electrodes is SiOx whose thickness is dp = 250 nm and dielectric constant is εp = 4.5 .
Figure 5c and Figure 4d depict the simulated equal-potential lines and LC director deformation in a voltage-on state of n-FFS and p-FFS, respectively. The cell is sandwiched between two crossed linear polarizers, and the transmission axis of the bottom polarizer is parallel to the rubbing direction. Thus, the transmittance at a given position and voltage V can be expressed as [39,45]:
3.3. Phase Retardation Effect
Both peak transmittance (Tp) and on-state voltage (Von) are dependent on the phase retardation, or dΔn/λ of the FFS cell. Figure 6 depicts the calculated Tp and Von at different dΔn/λ values for both n-FFS (with UCF-N1) and p-FFS (with UCF-P1). For n-FFS, as dΔn/λ increases from 0.35 to 1.1, Tp climbs to a peak of 98.1% at dΔn/λ ≈ 0.67 and then gradually decreases. Meanwhile, Von decreases to a minimum at dΔn/λ ≈ 0.7 and then bounces back. Since green light is the major component of white light, we optimize the cell gap at λ = 550 nm. Therefore, for n-FFS we choose dΔn ~ 360 nm for λ = 550 nm, in order to achieve high transmittance and fast response time. However, for p-FFS both Tp and Von increase continuously in the dΔn/λ range studied. The insufficient phase retardation results from the large tilt angle of the directors in the p-FFS (Figure 4b), because the positive Δε LC directors tend to align parallel to the electric fields. Compromising the performance between transmittance, Von and response time, we chose dΔn ~ 380 nm at λ = 550 nm as the optimal value for p-FFS.
An attractive feature of n-FFS can be found in Figure 5: in the 0.60 < dΔn/λ < 0.78 range Tp keeps larger than 95% and Von only varies slightly, which provides a reasonably large cell gap manufacturing tolerance. By contrast, in the same range the Von of p-FFS climbs almost linearly from 4 V to 5.2 V and Tp increases from 82% to 91.7%. Although the Tp of p-FFS gradually saturates when dΔn/λ > 0.7, its Von increases dramatically. High operation voltage leads to high power consumption.
3.4. Wavelength Effect
To achieve high transmittance, we optimize the cell gap for λ = 550nm. However, dΔn/λ varies for RGB colors due to the change in λ and birefringence dispersion as Figure 3 depicts. As Equation (5) indicates, a high birefringence LC is more dispersive in the visible region because of its longer λ*. Thus, the phase retardation for blue will be larger than the optimized value for green, but smaller for red. Larger birefringence dispersion causes a larger deviation from the optimized phase retardation value and hence leads to a lower peak transmittance. To investigate the birefringence dispersion effect on the transmittance for RGB (λ = 650, 550 and 450 nm) colors, we calculated the VT curves of n-FFS with three exemplary LCs: UCF-N0, UCF-N1 and UCF-N3, as shown in Figure 7a–c. UCF-N0 is an imaginary material; it has identical properties as UCF-N1 but without dispersion, i.e., its Δn is independent of wavelength. This represents an extreme case. On the other hand, UCF-N3 is a high birefringence negative Δε LC we developed for VA LCOS (to be discussed in next session), whose Δn = 0.177, 0.191 and 0.214 at RGB colors, respectively. For all the n-FFS cells studied, we set dΔn = 360 nm. Therefore for UCF-N0, its dΔn/λ = 0.55, 0.65 and 0.80 for RGB, respectively. From Figure 6, we find the peak transmittance for RGB is ~92%, 98% and 91%, which is consistent with the calculated VT curves of UCF-N0 for RGB colors, as depicted in Figure 7a. Moreover, both RGB colors have nearly the same Von. The inset in Figure 7a depicts the normalized VT curves and they overlap amazingly well. Thus, a single gamma curve driving can be realized for n-FFS, which would simplify the driving circuit. This property holds true for UCF-N1 and UCF-N3 as well. From Figure 5, Von is relatively insensitive to dΔn/λ in the range of 0.55–0.90. The peak transmittance of UCF-N1 reaches ~98% (λ = 550 nm) at Von = 4.6 V. As the birefringence dispersion gets larger, Tp(B) and Tp(R) drop further to 85% and 89% for UCF-N1, respectively. For UCF-N3, Tp(B) decreases to 71.3%, since dΔn/λ deviates from the optimized value too much. Tp(G) also drops slightly to 94% since the cell gap employed here is 1.89 μm, which is much smaller than the electrode width (3 μm). Fine electrode configuration  or adding chiral dopant  would help increase Tp for a thin-cell-gap FFF cell.
For comparison, we also calculate the VT curves of a p-FFS cell using UCF-P1 (d = 3.19 μm). Let’s call it FFS-P1. As Figure 7d shows, the peak transmittance of RGB colors take place at different voltages. For 550 nm, Tp reaches ~88% at Von = 4.4 V, and for 650 nm Tp reaches ~78% at Von = 4.0 V. But for λ = 450 nm, Tp can reach 88.1% but at a much higher voltage (6.8 V). The inset in Figure 7d depicts the normalized VT curves. Obviously, they do not overlap well. Thus, three different gamma curves are needed to drive the RGB pixels.
3.5. Director Deformation Distribution
In order to understand the differences between n-FFS and p-FFS modes, we study the LC tilt and twist angle distributions of FFS-N1 (n-FFS filled with UCF-N1) and FFS-P1 cells at five positions: A, B, C, D, and E as Figure 8a shows. Negative LCs tend to align perpendicular to the electric field, so the tilt angles at position A to E are relatively small, as shown in Figure 7a. To obtain maximum transmittance, ideally the twist angle should occur at 45°, as Equation (8) indicates. From Figure 8b, the LC directors are largely twisted near the bottom of the cell (z/d < 0.4) by the electric field and gradually reoriented back to the rubbing direction due to the strong anchoring force provided by the top surface. For FFS-N1, the maximum twist angle from the initial rubbing direction is around 46° at A and E. The tilt angle at A and E is close to 0, which contributes effectively to the phase retardation. At B, C, and D, the horizontal electric field is stronger and the maximum twist angle is ~55°. Meanwhile, the tilt angle at z/d ~ 0.1 is ~±10°, which would slightly decrease the phase retardation and compensate the over twist. Moreover, the on-state of the n-FFS cell is like two cascaded TN cells  due to the small tilt angle. As a result, polarization rotation effect dominates and the color dispersion is suppressed.
In contrast, the maximum twist angle of FFS-P1 is either larger than 63° (B and C) or smaller than 38° (A and E), as Figure 7d depicts. The over- or under-twist leads to inefficient phase retardation. Only at position D, the maximum twist angle is about 48°, however the tilt angle is about 41° at z/d = 0.1. The large tilt angle (Figure 7c) caused by the strong vertical field dramatically decreases the effective birefringence and hence the peak transmittance. Meanwhile, with a large tilt angle at positions B, C, and D, the phase retardation effect (which is wavelength sensitive) becomes quite obvious, resulting in severe wavelength dispersion. In addition, from Figure 5d, splay and bend deformation occurs and electric polarization is induced, which is known as flexoelectric effect . The light transmittance would change slightly from negative to positive frames, resulting in a small image flickering. By contrast, this effect is negligible in n-FFS due to the small tilt angle.
As Figure 7 shows, FFS-P1 has a lower threshold-like voltage (Vth) than FFS-N1 because its Δε (+10) is much larger than that of UCF-N1 (−3.82), assuming their K22 is the same. However, the on-state voltage of FFS-P1 (Von ~ 4.4 V) is nearly the same as that of FFS-N1 (4.6 V). This can be explained by the LC director distributions shown in Figure 8a–d. FFS-N1 has more efficient twist angle (~45°) and smaller tilt angle than FFS-P1 so that its effective birefringence is higher. As a result, a smaller voltage swing (ΔV = Von − Vth) is needed to reach the peak transmittance. Therefore, FFS-N1 has a comparable Von to FFS-P1, although its Δε is much smaller.
3.6. Low Operation Voltage
Low power consumption is highly desirable for a mobile display because it lengthens the battery life. The power consumption of a LCD comes from two parts: electronic and backlight. Generally speaking, the total power consumption is governed by the optical throughput of the panel, circuit frame rate, capacitance, and square of the operation voltage. For a given resolution and frame rate, the power consumption is closely related to the optical efficiency and operation voltage.
Several approaches have been considered for lowering Von. From device side, we can decrease the rubbing angle [45,46]. The tradeoff is slower rise time, although the decay time remains almost the same. In FFS mode, the capacitor formed by the passivation layer between the pixel and common electrode acts as a storage capacitor (Cs ~ εpApixel/dp), which is in parallel to the LC capacitor. Therefore, we can use a thin and large εp dielectric layer to increase Cs and reduce the voltage shielding effect . For example, if we reduce the SiOx layer thickness from 250 nm to 100 nm, then Von would decrease from 4.6 V to 3.9 V for FFS-N1. If we use 100 nm Si3N4 passivation layer (εp = 6.5), then Von would drop to 3.8 V. A tradeoff is the increased charging time resulting from the increased Cs. However, for a high resolution mobile display, its pixel size is small so that Cs can still be kept relatively small for quick addressing.
From material aspect, a straightforward way to reduce Von is to increase Δε. As shown in Figure 9, as Δε increases, the Von of n-FFS decreases dramatically initially and then gradually saturates for both 250-nm SiOx layer (solid circle) and 100-nm Si3N4 layer (open circle). The two sets of data points are well fitted by the following semi-empirical equation:
3.7. Response Time
Both rise time and decay time are calculated between the 10% and 90% transmittance change. For FFS-P1 with d = 3.19 μm, the simulated [rise time, decay time] is [23.8 ms, 25.7 ms]. For the n-FFS cell with MLC-6882 (d = 3.66 μm and Von = 4.5 V) the simulated [rise time, decay time] is [23.4 ms, 34.8 ms]. With our UCF-N1 (d = 3.02 μm), the calculated [rise time, decay time] is [16.2 ms, 24.1 ms]. Our UCF-N1 has faster response time than MLC-6882 because of its thinner cell gap. On the other hand, UCF-N1 has faster response time than FFS-P1 due to its more uniform twist and tilt angles. A lower viscosity LC would further reduce the response time. For example, if we use a lower viscosity LC, such as UCF-N2, the calculated [rise time, decay time] decreases about 30% to [10.9 ms, 16.5 ms].
This response time is still 2X to 3X longer than that of the state-of-the-art MVA LCD TV. In MVA, the involved elastic constant is K33, but in n-FFS it is K22. For most nematic LCs, K33 is about 2X to 3X larger than K22. Therefore, this could be an intrinsic disadvantage when comparing n-FFS with MVA for TV applications, where touch panel is not necessary. To further improve the response time for n-FFS, we need to develop lower viscosity negative Δε LCs or use a thinner cell gap.
We have developed a low viscosity negative Δε LC mixture (UCF-N2, γ1 = 94 mPas and Δn ~ 0.12) for n-FFS with a 3-μm cell gap. Our n-FFS shows superior performances to p-FFS in following aspects: (1) higher transmittance (98% vs. 88%); (2) single gamma curve vs. 3 gamma curves for RGB pixels; (3) both on-state voltage and peak transmittance are less sensitive to cell gap variation, (4) faster response time due to a slightly thinner cell gap and more uniform LC twist and tilt angles, and (5) comparable on-state voltage to p-FFS although the LC mixture has a smaller Δε (−3.8 vs. +10). Therefore, n-FFS has potential to replace p-FFS for next-generation mobile displays or even TV applications. Moreover, due to the homogeneous alignment and horizontal molecular orientation, n-FFS has intrinsic wide viewing angles. Various compensation films for FFS mode have been developed [49,50]. With one biaxial film, the 100:1 isocontrast contour can be achieved over the ±80° viewing zone . To further widen the viewing angle, multi-domain structures can be considered .
4. Negative Δε LCs for VA Mode
Two types of VA cells are discussed here: single domain VA LCOS for projection displays and multi-domain VA (MVA) for direct-view LCD TVs.
Single domain VA has been extensively used in LCOS for projection displays because of its unprecedented contrast ratio (CR) . To enable color sequential projection display [51,52,53], which requires only a single monochrome LCD panel so that the optical system is much simpler than that using three panels, fast response time (<1 ms) is critically needed in order to suppress color breakup. To achieve submillisecond response time, several approaches have been proposed, such as thin VA LCOS cell [18,19], mixed-mode twisted nematic (MTN) cell  and ferroelectric cell . Among these methods, thin VA LCOS is attractive because of its high CR and fast response time, as shown in Equation (3). However, fringing field degrades the contrast ratio and reduces the display brightness . A straightforward way to suppress fringing field effect is to reduce the cell gap. A major challenge for the thin cell approach is the need of a high birefringence and low viscosity LC. For a VA LCOS, the required dΔn is ~165 nm (at λ = 550 nm) in order to achieve high reflectance at a low voltage (<5 V) .
In projection displays, high power arc lamp or LED lamp is commonly used as light source. Because of thermal effect, the LCOS panel is usually operated at 40–50 °C. As the temperature increases, both birefringence and visco-elastic coefficient decrease. The former vanishes at Tc. Therefore, it is important to design a LC with high Tc (>>50 °C). In an LCOS, the electric field is in the longitudinal direction. To realize the electro-optic effect of a VA cell, we need a negative Δε LC. To achieve high resistivity, fluorinated LCs are commonly used as mentioned earlier . However, some laterally difluoro high Δn compounds are difficult to align, especially at elevated temperatures . A poor LC alignment leads to a low contrast ratio.
UV stability is another critical issue for a high Δn LC due to its relatively long conjugation length. In an LCOS projector, the arc lamp is relatively bright. Although filters are used to block the unwanted UV and infrared lights from the lamp, residual UV contents could still decompose the LC materials if the molecular structures are not intrinsically stable.
4.1.1. LC Material
In experiment, we prepared a mixture called UCF-N3 by doping 15.1 wt % lateral difluoro alkoxy-biphenyls, 8.9 wt % alkoxy-cyclohexane-phenyls, and 15.4 wt % alkoxy-cyclohexane-biphenyls [9,58], whose chemical structures are shown in Figure 1, into our M1 host in order to increase Δε while keeping a low viscosity. An excellent dark state was achieved in the entire nematic range. The clearing point of UCF-N3 is Tc ~ 93.2 °C.
4.1.2. Physical Properties
We first measured the dielectric anisotropy of UCF-N3 at f = 1 kHz. Results are: Δε = −3.74 at 23 °C and −2.91 at 50 °C. Next, we measured the temperature dependent Δn of UCF-N3 at λ = 633 nm from 25 °C to 90 °C. Results are plotted in Figure 10a, where dots represent the measured data and solid line is the fitting curve using Equation (4). Through fitting, we obtained Δn0 = 0.265 and β = 0.177.
To investigate the electro-optic performances at RGB colors, we measured the birefringence dispersion of UCF-N3 at 50 °C; the intended operation temperature for an LCOS projector. Results are shown in Figure 10b; here dots are the measured data and solid line represents fitting result using Equation (5). From fitting we obtained G = 2.64E-6 μm−2 and λ* = 241.1 nm. With higher Δn, UCF-N3 has a longer λ* than the previously mentioned mixtures for FFS. With these parameters and through Equation (5), we can obtain the birefringence at any wavelength. For example, we find Δn = 0.191 at λ = 550 nm and 50 °C. Thus, for a VA LCOS we need d = 0.93 μm to achieve ~100% reflectance (normalized to parallel polarizers) at a relatively low operating voltage (<5 V). Although challenging, ferroelectric LCOS with d ~ 0.8 μm has been commercialized.
We also measured the γ1/K33 of UCF-N3 at different temperatures and fitted the experimental data with Equation (6), as shown in Figure 11a. Here the activation energy is Ea = 286.9 meV, which is larger than that of UCF-N2 developed for FFS. Usually higher birefringence involves longer conjugation length and hence higher viscosity, which leads to larger activation energy. To evaluate the overall performance of UCF-N3 at different temperatures, Figure 11b depicts the measured FoM data and fitting curve based on Equation (7). At room temperature, the FoM of UCF-N3 is ~2.6 μm2/s, and it increases to 4.8 μm2/s at 50 °C.
4.1.3. Simulation Results for VA LCOS
The electro-optical characteristics of UCF-N3 in a vertical alignment liquid-crystal-on-silicon (VA-LCOS) are calculated using a commercial LCD simulator DIMOS 2.0. In simulation, we used d = 0.93 μm, Δn = 0.191 at λ = 550 nm, and γ1/K33 ~ 6.7 ms/μm2 at T = 50 °C. The initial pretilt angle is 88° and the azimuthal angle is 45° w.r.t. the optic axis of the polarizing beam splitter (PBS). A reflector is placed on the inner surface of the VA cell. We calculated the voltage-dependent reflectance (VR) curves for RGB colors. As shown in Figure 12, for the green light the on-state voltage occurs at 4.83 V. The birefringence dispersion is relatively large for high birefringence LCs. As shown in Figure 10b, Δn = 0.214, 0.191, 0.177 at λ = 450 nm, 550 nm and 650 nm, respectively. The peak transmittance for RGB colors occur at different voltages. Thus, three gamma curves are needed for driving the RGB sub-frames.
We also calculated the gray-to-gray (GTG) response times of the VA LCOS, and results are summarized in Table 2. Taking green color as an example, the VR curve was uniformly divided into eight gray levels (1–8) and the response time between every two gray levels was calculated. Here both rise time and decay time are calculated between 10% and 90% reflectance change. From Table 2, we find the rise time is 0.26 ms and decay time is 0.40 ms between gray levels 1 and 8. The average GTG rise time is 0.75 ms and decay time is 0.79 ms. With such a fast response time, image blur and color breakup can be greatly suppressed.
|Table 2. Calculated GTG response time (unit: ms) of the UCF-N3 VA LCOS at 50 °C. d = 0.93 μm.|
The estimated operation temperature range for the proposed color sequential VA-LCOS is from 20 °C to 70 °C. As the operation temperature decreases, the response time would be slower because of the increased γ1/K33. For example, if the application is at room temperature, then from Figure 11a the estimated response time would be ~2.3X slower than that at 50 °C. To shorten response time, overdrive and undershoot voltage method can be applied. On the other hand, if the operation temperature exceeds 70 °C, then the birefringence decreases noticeably as Figure 10 depicts. As a result, the optical efficiency will decline because the phase retardation is less than 1π.
4.1.4. UV Stability
As mentioned above, UV stability is an important concern for an arc-lamp-based LCOS projector. UV light could damage the polyimide alignment layers and the LC material . To investigate UV stability, we exposed our UCF-N3 cell (ITO glass substrates) with a UV LED lamp (λ ~ 385nm and light intensity ~300 mW/cm2) for five hours. After UV exposure, UCF-N3 shows no sign of degradation: clearing point, dark state, threshold voltage, and electro-optic properties all remain unchanged within the experimental error.
For a high pressure Mercury arc lamp, the emission spectrum contains some harmful UV components in the 380–400 nm range. Therefore, a UV filter with cutoff wavelength ~420 nm is commonly employed. With such a UV filter, our LC mixture should have an excellent stability. For a typical RGB LED backlight unit, its UV content is negligible.
Our fluorinated high birefringence, low viscosity and negative Δε LC mixture UCF-N3 enables a VA LCOS to achieve high contrast ratio, low voltage, and submillisecond GTG response time at an elevated temperature. Such a fast response time enables color sequential display using a single monochrome LCD panel. As a result, the optical system is greatly simplified. Moreover, good UV stability makes this LC mixture practical for projection displays. A thin cell gap (0.93 μm) also helps to suppress fringing field effect. Although making a submicron cell gap is technically challenging, it has been done in ferroelectric LCOS devices.
4.2. MVA Mode
For wide-view LCD TVs, MVA [20,60,61,62] and multi-domain IPS [49,63] are the two major approaches. In a transmissive MVA LCD, the required dΔn is 330 nm (at λ = 550 nm) for achieving high transmittance and low driving voltage. The cell gap currently employed is around 3–4 μm. Thus, a low viscosity negative Δε LC with Δn ~ 0.08–0.11 is commonly used. These LC mixtures are commercially available. For a 3-μm cell gap, the response time is about 4–5 ms. As the manufacturing technology continues to advance, a thinner cell gap could be used in the near future for reducing response time. For example, if the cell gap can be reduced to 2.5 μm, then the response time would be improved by ~40%, however, the required Δn should be increased to 0.13. Our low viscosity UCF-N2 (Δn ~ 0.12) can be considered for MVA applications as well, in addition to n-FFS.
If we keep the cell gap at 3-μm for our UCF-N2, then the on-state voltage is ~5.6 V, as Figure 13 shows. On the other hand, if we use MLC 6882 and keep dΔn = 330 nm at λ = 550 nm (d = 3.37 μm), then its Von ~ 7.6 V. Low voltage helps to reduce power consumption.
We have reviewed recent progress on the development of negative Δε LCs for FFS and VA display applications. With our UCF-N2, n-FFS shows superior performance to p-FFS in high transmittance, single gamma curve, cell gap insensitivity, and negligible flexoelectric effect. Using our UCF-N3 for VA LCOS, we have demonstrated a submillisecond gray-to-gray response time for color sequential projection displays. Our low viscosity UCF-N2 can also be used for MVA LCD TVs
This work is partially supported by AFOSR under contract No. FA95550-09-1-0170.
Conflicts of Interest
The authors declare no conflict of interest.
- Kirsch, P.; Heckmeier, M.; Tarumi, K. Design and synthesis of nematic liquid crystals with negative dielectric anisotropy. Liq. Cryst. 1999, 26, 449–452, doi:10.1080/026782999205236.
- Kirsch, P.; Reiffenrath, V.; Bremer, M. Nematic liquid crystals with negative dielectric anisotropy: Molecular design and synthesis. Synlett 1999, 1999, 389–396, doi:10.1055/s-1999-2619.
- Klasen, M.; Bremer, M.; Tarumi, K. New liquid-crystal materials for active matrix displays with negative dielectric anisotropy and low rotational viscosity. Jpn. J. Appl. Phys. 2000, 39, L1180–L1182, doi:10.1143/JJAP.39.1180.
- Kirsch, P.; Tarumi, K. A novel type of liquid crystals based on axially fluorinated cyclohexane units. Angew. Chem. Int. Ed. 1998, 37, 484–489, doi:10.1002/(SICI)1521-3773(19980302)37:4<484::AID-ANIE484>3.0.CO;2-6.
- Schadt, M. Liquid crystal materials and liquid crystal displays. Annu. Rev. Mater. Sci. 1997, 27, 305–379, doi:10.1146/annurev.matsci.27.1.305.
- Hird, M.; Goodby, J.W.; Toyne, K.J. Nematic materials with negative dielectric anisotropy for display applications. Proc. SPIE 2000, 3955, 15–23, doi:10.1117/12.379979.
- Ogata, M.; Ukai, K.; Kawai, T. Visual fatigue in congenital nystagmus caused by viewing images of color sequential projectors. J. Disp. Technol. 2005, 1, 314–320, doi:10.1109/JDT.2005.858918.
- Chen, Y.; Sun, J.; Xianyu, H.; Wu, S.T.; Liang, X.; Tang, H. High birefringence fluoro-terphenyls for thin-cell-gap TFT-LCDs. J. Disp. Technol. 2011, 7, 478–481, doi:10.1109/JDT.2011.2150197.
- Hird, M. Fluorinated liquid crystals—Properties and applications. Chem. Soc. Rev. 2007, 36, 2070–2095, doi:10.1039/b610738a.
- Gray, G.W.; Hird, M.; Toyne, K.J. The synthesis of several lateral difluoro-substituted 4,4′′-dialkyl- and 4,4′′-alkoxyalkyl-terphenyls and a rationalisation of the effect of such substitution on mesophase type and transition temperatures. Mol. Cryst. Liq. Cryst. 1991, 204, 43–64, doi:10.1080/00268949108046593.
- Wu, S.T.; Hsu, C.S.; Chen, J.M. Room temperature difluoro-tolane and diphenyl-diacetylene liquid crystals with negative dielectric anisotropy. Mol. Cryst. Liq. Cryst. 1997, 304, 441–445, doi:10.1080/10587259708046994.
- Li, Y.; Chen, Y.; Yan, J.; Liu, Y.; Cui, J.; Wang, Q.; Wu, S.T. Polymer-stabilized blue phase liquid crystal with a negative Kerr constant. Opt. Mater. Express 2012, 2, 1135–1140, doi:10.1364/OME.2.001135.
- Ge, Z.; Zhu, X.; Wu, T.X.; Wu, S.T. High transmittance in-plane switching liquid crystal displays. J. Disp. Technol. 2006, 2, 114–120, doi:10.1109/JDT.2006.874502.
- Oh-e, M.; Kondo, K. Electro-optical characteristics and switching behavior of the in-plane switching mode. Appl. Phys. Lett. 1995, 67, 3895–3897, doi:10.1063/1.115309.
- Lee, S.H.; Lee, S.L.; Kim, H.Y. Electro-optic characteristics and switching principle of a nematic liquid crystal cell controlled by fringe-field switching. Appl. Phys. Lett. 1998, 73, 2881–2883, doi:10.1063/1.122617.
- Chen, Y.; Luo, Z.; Peng, F.; Wu, S.T. Fringe-field wwitching with a negative dielectric anisotropy liquid crystal. J. Disp. Technol. 2013, 9, 74–77, doi:10.1109/JDT.2013.2242844.
- Yun, H.J.; Jo, M.H.; Jang, I.W.; Lee, S.H.; Ahn, S.H.; Hur, H.J. Achieving high light efficiency and fast response time in fringe field switching mode using a liquid crystal with negative dielectric anisotropy. Liq. Cryst. 2012, 39, 1141–1148, doi:10.1080/02678292.2012.700078.
- Schiekel, M.F.; Fahrenschon, K. Deformation of nematic liquid crystals with vertical orientation in electrical fields. Appl. Phys. Lett. 1971, 19, 391–393, doi:10.1063/1.1653743.
- Kahn, F.J. Electric-field-induced orientational deformation of nematic liquid-crystals: Tunable birefringence. Appl. Phys. Lett. 1972, 20, 199–201, doi:10.1063/1.1654107.
- Takeda, A.; Kataoka, S.; Sasaki, T.; Chida, H.; Tsuda, H.; Ohmuro, K.; Sasabayashi, T.; Koike, Y.; Okamoto, K. A super-high image quality multi-domain vertical alignment LCD by new rubbing-less technology. SID Symp. Dig. Tech. Pap. 1998, 29, 1077–1080, doi:10.1889/1.1833672.
- Ohmuro, K.; Kataoka, S.; Sasaki, T.; Koike, Y. Development of super-high-image-quality vertical-alignment-mode LCD. SID Int. Symp. Dig. Tech. Pap. 1997, 28, 845–850.
- Cuypers, D.; De Smet, H.; Van Calster, A. VAN LCOS microdisplays: A decade of technological evolution. J. Disp. Technol. 2011, 7, 127–134, doi:10.1109/JDT.2010.2053018.
- Khoo, I.C.; Wu, S.T. Optics and Nonlinear Optics of Liquid Crystals; World Scientific: Singapore, 1993.
- Yang, D.K.; Wu, S.T. Fundamentals of Liquid Crystal Devices; Wiley: New York, NY, USA, 2006.
- Wu, S.T.; Wu, C.S. Small angle relaxation of highly deformed nematic liquid crystals. Appl. Phys. Lett. 1988, 53, 1794–1796, doi:10.1063/1.99783.
- Xu, D.; Rao, L.; Tu, C.-D.; Wu, S.-T. Nematic liquid crystal display with submillisecond grayscale response time. J. Disp. Technol. 2013, 9, 67–70, doi:10.1109/JDT.2012.2232902.
- Wu, S.T. Nematic liquid crystal modulator with response time less than 100 μs at room temperature. Appl. Phys. Lett. 1990, 57, 986–988, doi:10.1063/1.103533.
- Wu, S.T.; Margerum, J.D.; Meng, H.B.; Dalton, L.R.; Hsu, C.S.; Lung, S.H. Room-temperature diphenyl-diacetylene liquid-crystals. Appl. Phys. Lett. 1992, 61, 630–632, doi:10.1063/1.107829.
- Wu, S.T.; Hsu, C.S.; Shyu, K.F. High birefringence and wide nematic range bis-tolane liquid crystals. Appl. Phys. Lett. 1999, 74, 344–346, doi:10.1063/1.123066.
- Sekine, C.; Fujisawa, K.; Iwakura, K.; Minai, M. High birefringence phenylacetylene liquid crystals with low viscosity. Mol. Cryst. Liq. Cryst. 2001, 364, 711–718, doi:10.1080/10587250108025039.
- Gauza, S.; Jiao, M.; Wu, S.T.; Kula, P.; Dąbrowski, R.; Liang, X. High birefringence and low viscosity negative dielectric anisotropy liquid crystals. Liq. Cryst. 2008, 35, 1401–1408, doi:10.1080/02678290802624381.
- Lee, S.H.; Lee, S.M.; Kim, H.Y.; Kim, J.M.; Hong, S.H.; Jeong, Y.H.; Park, C.H.; Choi, Y.J.; Lee, J.Y.; Koh, J.W. Ultra-FFS TFT-LCD with Super Image Quality and Fast Response Time. SID Symp. Dig. Tech. Pap. 2001, 32, 484–487, doi:10.1889/1.1831901.
- Lee, S.H.; Lee, S.L.; Kim, H.Y.; Eom, T.Y. A novel wide-viewing-angle technology: Ultra-Trans View™. SID Symp. Dig. Tech. Pap. 1999, 30, 202–205, doi:10.1889/1.1833995.
- Blinov, L.M.; Chigrinov, V.G. Electrooptic Effects in Liquid Crystal Materials; Springer-Verlag: New York, NY, USA, 1994.
- Lee, J.H.; Park, K.H.; Kim, S.H.; Choi, H.C.; Kim, B.K.; Yin, Y. AH-IPS: Superb display for mobile device. SID Symp. Dig. Tech. Pap. 2013, 44, 32–33, doi:10.1002/j.2168-0159.2013.tb06132.x.
- Wen, C.H.; Gauza, S.; Wu, S.T. High-contrast vertical alignment of lateral difluoro-terphenyl liquid crystals. Appl. Phys. Lett. 2005, 87, 191909:1–191909:3, doi:10.1063/1.2128068.
- Clark, M.G.; Raynes, E.P.; Smith, R.A.; Tough, R.J.A. Measurement of the permittivity of nematic liquid-crystals in magnetic and electric-fields using extrapolation procedures. J. Phys. D Appl. Phys. 1980, 13, 2151:1–2151:11.
- Wu, S.T.; Wu, C.S. Experimental confirmation of the Osipov-Terentjev theory on the viscosity of nematic liquid-crystals. Phys. Rev. A 1990, 42, 2219–2227, doi:10.1103/PhysRevA.42.2219.
- Wu, S.T.; Efron, U.; Hess, L.D. Birefringence measurements of liquid-crystals. Appl. Opt. 1984, 23, 3911–3915, doi:10.1364/AO.23.003911.
- Haller, I. Thermodynamic and static properties of liquid crystals. Prog. Solid State Chem. 1975, 10, 103–118, doi:10.1016/0079-6786(75)90008-4.
- Wu, S.T. Birefringence dispersions of liquid-crystals. Phys. Rev. A 1986, 33, 1270–1274, doi:10.1103/PhysRevA.33.1270.
- Wu, S.T.; Lackner, A.M.; Efron, U. Optimal operation temperature of liquid-crystal modulators. Appl. Opt. 1987, 26, 3441–3445, doi:10.1364/AO.26.003441.
- Lien, A. Extended Jones Matrix representation for the twisted nematic liquid-crystal display at oblique-incidence. Appl. Phys. Lett. 1990, 57, 2767–2769, doi:10.1063/1.103781.
- Ge, Z.B.; Wu, S.T.; Kim, S.S.; Park, J.W.; Lee, S.H. Thin cell fringe-field-switching liquid crystal display with a chiral dopant. Appl. Phys. Lett. 2008, 92, 181109:1–181109:3.
- Hong, S.H.; Park, I.C.; Kim, H.Y.; Lee, S.H. Electro-optic characteristic of fringe-field switching mode depending on rubbing direction. Jpn. J. Appl. Phys. 2000, 39, L527–L530.
- Sun, Y.; Zhang, Z.; Ma, H.; Zhu, X.; Wu, S.T. Optimal rubbing angle for reflective in-plane-switching liquid crystal displays. Appl. Phys. Lett. 2002, 81, 4907–4909, doi:10.1063/1.1532534.
- Jiao, M.; Ge, Z.; Song, Q.; Wu, S.T. Alignment layer effects on thin liquid crystal cells. Appl. Phys. Lett. 2008, 92, 061102:1–061102:3.
- Hatsumi, R.; Kubota, Y.; Moriya, K.; Kubota, D.; Tanabe, T.; Kusunoki, K.; Hirakata, Y.; Koyama, J.; Yamazaki, S.; Nakamura, A.; Chubachi, Y. Driving method of FFS-Mode OS-LCD for reducing eye strain. SID Symp. Dig. Tech. Pap. 2013, 44, 338–341, doi:10.1002/j.2168-0159.2013.tb06215.x.
- Lu, R.; Zhu, X.; Wu, S.T.; Hong, Q.; Wu, T.X. Ultrawide-view liquid crystal displays. J. Disp. Technol. 2005, 1, 3–14, doi:10.1109/JDT.2005.852507.
- Zhu, X.; Ge, Z.; Wu, S.T. Analytical solutions for uniaxial-film-compensated wide-view liquid crystal displays. J. Disp. Technol. 2006, 2, 2–20, doi:10.1109/JDT.2005.863599.
- Armitage, D.; Underwood, I.; Wu, S.T. Introduction to Miscrodisplay; Wiley: Hoboken, NJ, USA, 2006.
- Brennesholtz, M.S.; Stupp, E.H. Projection Displays; Wiley: Chichester, UK, 2008.
- Gauza, S.; Zhu, X.; Piecek, W.; Dabrowski, R.; Wu, S.T. Fast switching liquid crystals for color-sequential LCDs. J. Disp. Technol. 2007, 3, 250–252, doi:10.1109/JDT.2007.900909.
- Wu, S.T.; Wu, C.S. Mixed-mode twisted nematic liquid crystal cells for reflective displays. Appl. Phys. Lett. 1996, 68, 1455–1457, doi:10.1063/1.116252.
- Lee, S.; Mao, C.C.; Johnson, K.M. Fast-switching liquid-crystal-on-silicon microdisplay with Framebuffer pixels and surface-mode optically compensated birefringence. Opt. Eng. 2006, 45, 127402:1–127402:8.
- Fan-Chiang, K.H.; Wu, S.T.; Chen, S.H. Fringing-field effects on high-resolution liquid crystal microdisplays. J. Disp. Technol. 2005, 1, 304–313, doi:10.1109/JDT.2005.858930.
- Wang, H.; Wu, T.X.; Zhu, X.; Wu, S.T. Correlations between liquid crystal director reorientation and optical response time of a homeotropic cell. J. Appl. Phys. 2004, 95, 5502–5508, doi:10.1063/1.1707210.
- Chen, Y.; Peng, F.; Wu, S.T. Submillisecond-response vertical-aligned liquid crystal for color sequential projection displays. J. Disp. Technol. 2013, 9, 78–81, doi:10.1109/JDT.2013.2243403.
- Wen, C.H.; Gauza, S.; Wu, S.T. Photostability of liquid crystals and alignment layers. J. Soc. Inf. Disp. 2005, 13, 805–811, doi:10.1889/1.2080522.
- Kim, S.S. The world’s largest (82-in) TFT-LCD. SID Symp. Dig. Tech. Pap. 2005, 36, 1842–1847, doi:10.1889/1.2036378.
- Miyachi, K.; Kobayashi, K.; Yamada, Y.; Mizushima, S. The world’s first photo alignment LCD technology applied to Generation Ten factory. SID Symp. Dig. Tech. Pap. 2010, 41, 579–582, doi:10.1889/1.3500533.
- Lee, S.H.; Kim, S.M.; Wu, S.T. Emerging vertical-alignment liquid-crystal technology associated with surface modification using UV-curable monomer. J. Soc. Inf. Disp. 2009, 17, 551–559, doi:10.1889/JSID17.7.551.
- Hong, H.; Shin, H.; Chung, I. In-plane switching technology for liquid crystal display television. J. Disp. Technol. 2007, 3, 361–370, doi:10.1109/JDT.2007.901562.
© 2013 by the authors; licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution license (http://creativecommons.org/licenses/by/3.0/).